Harper CZM

Upload
nicolemcdonald 
Category
Documents

view
224 
download
0
Embed Size (px)
Transcript of Harper CZM

8/11/2019 Harper CZM
1/19
Cohesive zone length in numerical simulations of composite delamination
Paul W. Harper, Stephen R. Hallett *
Advanced Composites Centre for Innovation and Science, University of Bristol, Queens Building, University Walk, Bristol BS8 1TR, UK
a r t i c l e i n f o
Article history:Received 21 December 2007Received in revised form 1 May 2008Accepted 16 June 2008Available online 26 June 2008
Keywords:CompositesDelaminationInterface fractureFinite element analysisCohesive zone modelling
a b s t r a c t
Accurate analysis of composite delamination using interface elements relies on having suf
cient elements within a softening region known as the cohesive zone ahead of a crack tip.The present study highlights the limitations of existing formulae used to predict numericalcohesive zone length and demonstrates modications necessary for improved accuracy.Clarication is also provided regarding the minimum number of interface elements withinthe cohesive zone. Finally, appropriate values of numerical interfacial strength are examined. The results presented will aid the application of mesh design techniques that bothpreserve numerical accuracy, whilst minimising computational expense.
2008 Elsevier Ltd. All rights reserved.
1. Introduction and motivation
Interface elements are specialised nite elements used to simulate crack initiation and propagation in numerical models.Over recent years, they have become increasingly used for modelling composites, particularly in relation to delamination [17] and adhesive bondline failure [811] . Compared with alternative analysis techniques such as the virtual crack closuretechnique (VCCT), they offer the advantages of encompassing both crack initiation and crack propagation and the abilityto model multiple crack paths, without the need for computationally expensive crackpath following algorithms. In addition,they do not require the direction of crack propagation to be known in advance, and cracks have the potential to propagatealong any path where interface elements are placed [2] . Fig. 1 demonstrates a typical simulation of composite delaminationin a mode I double cantilever beam (DCB).
An interface elements behaviour is governed by a tractiondisplacement curve, relating element stress (traction) to modeI (opening) and mode II (shear) nodal displacements. Although a variety of geometric shapes have been used for this tractiondisplacement curve, a bilinear form is commonly implemented for modelling composite delamination (see Fig. 2). Thisconsists of the following main features:
1. An initial elastic region until reaching a maximum stress ( r max ), which represents the interfacial strength.2. A subsequent softening region until zero stress is reached and element failure occurs.3. The total area enclosed by the curve is equal to the fracture toughness of the material.
Ahead of a numerical crack tip, we can dene a region known as the cohesive zone, in which elements experience irreversible deformation (i.e. region d ed f on the traction displacement response shown in Fig. 2). Fig. 3 illustrates the development of this zone, using the simple example of a mode I DCB specimen subject to a linearly increasing tip displacement. As
00137944/$  see front matter 2008 Elsevier Ltd. All rights reserved.doi:10.1016/j.engfracmech.2008.06.004
* Corresponding author.Email address: [email protected] (S.R. Hallett).
Engineering Fracture Mechanics 75 (2008) 47744792
Contents lists available at ScienceDirect
Engineering Fracture Mechanics
j o u r n a l h o m e p a g e : w w w. e l s e v i e r. c o m / l o c at e / e n g f r a c m e c h
mailto:[email protected]://www.sciencedirect.com/science/journal/00137944http://www.elsevier.com/locate/engfracmechhttp://www.elsevier.com/locate/engfracmechhttp://www.sciencedirect.com/science/journal/00137944mailto:[email protected] 
8/11/2019 Harper CZM
2/19
displacement initially increases, the interface element adjacent to the crack tip rapidly reaches its maximum interfacialstrength and moves onto the softening region of the tractiondisplacement response. As tip displacement increases further,adjacent elements also undergo irreversible deformation, allowing a cohesive zone length, LCZ, to be dened, over whichstress increases up to the maximum interfacial strength some distance ahead of the crack tip. The length of the cohesive zonereaches a maximum, LCZ,f , at the point where the crack tip interface element fails completely and the crack starts topropagate.
It is important to draw a clear distinction between the true physical cohesive zone length, dened as the length overwhich irreversible damage processes occur ahead of a crack tip and the numerical cohesive zone length, over which interface
Nomenclature
Interface element propertiesG strain energy release rate (N/mm)GC critical strain energy release rate (N/mm)K interface element stiffness prior to damage initiation (N/mm 3)r interface element stress (MPa)r max interfacial strength (MPa)d interface element relative displacement (mm)d e interface element relative displacement at damage initiation (mm)d f interface element relative displacement at nal failure (mm)
Laminate material propertiesE 11 , E 22 , E 11 Youngs moduli (MPa)G12 , G13 , G23 Shear moduli (MPa)m12 , m13 , m23 Poissons ratios, where subscripts 1, 2 and 3 denote the principal material axes
Laminate geometric propertiesh laminate half thickness (mm)B laminate width (mm)
X specimen length (mm)a crack length (mm)a0 initial crack length prior to crack propagation (mm)I second moment of area (mm 4)
OthersP load (N)D cantilever tip displacement (mm)lch characteristic cohesive zone length in an innite body (mm)lch,slender characteristic cohesive zone length in a slender body (mm)E
0equivalent elastic modulus used in the characteristic length equation for orthotropic materials (MPa)
LCZ numerical cohesive zone length (mm)LCZ,f fully developed numerical cohesive zone length (mm)N el number of elements within the numerical cohesive zone
Lel element length (mm)where applicable, subscripts I, II and m are used to denote properties under mode I, mode II and mixedmodeloading, respectively
Failed Interface Elements
New Crack Tip
Solid interface elementsplaced along potentialdelamination path
Initial Crack TipFailed Interface Elements
New Crack Tip
Solid interface elementsplaced along potentialdelamination path
Initial Crack TipFailed Interface Elements
New Crack Tip
P
Solid interface elementsplaced along potentialdelamination path
P
PInitial Crack Tip
P
Fig. 1. Interface element analysis of delamination in a double cantilever beam.
P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792 4775

8/11/2019 Harper CZM
3/19
elements lie on the softening part of their tractiondisplacement response. For an accurate numerical representation of thephysical cohesive zone, the shape of the tractiondisplacement curve must reect the stress distribution associated withdamage mechanisms occurring ahead of the physical crack tip [13] . However, this stress distribution is very difcult to measure experimentally and, if only a global analysis of the structures loaddisplacement response is required, results are relatively insensitive to the exact shape of the tractiondisplacement curve, provided that the correct interfacial strength andfracture toughness are applied [12] . This explains why the bilinear tractiondisplacement curve, which is geometrically themost simple form to implement, has become commonly used for delamination analyses [57] . Furthermore, once a crack has
initiated in a structure and a cohesive zone exists, results are relatively insensitive to the exact value of interfacial strengthand only the fracture toughness value is of critical importance [14] .
0
e
f
0 e : Elastic Deformation
I max
I e0
I I max
I e0
e f : Linear Softening
0 e
f
G IC
0
e
0 e :
I max
I e0
I I max
I e0
e f :
0 e0 e
f
f
G IC
Fig. 2. Bilinear tractiondisplacement response.
P
P
Global ForceDisplacementResponse
Crack Tip
x
Displacement ( )
2 3 4 51
x
LCZ
max F
o r c e
( P )
x
2 3 4 51
max
LCZ for crit(LCZ,f )
P crit
crit
CrackPropagation
Crack Tip Stress Distribution
P
P
Global ForceDisplacementResponse
Crack Tip
x
Displacement ( )
2 3 4 51
x
LCZ
max
2 3 4 51
x
LCZ
max F
o r c e
( P )
x
2 3 4 51
max
LCZ for crit(LCZ,f )
P crit
crit
CrackPropagation
Crack Tip Stress Distribution
Fig. 3. Development of the numerical cohesive zone.
4776 P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792

8/11/2019 Harper CZM
4/19
In order to conduct an accurate delamination analysis, the mesh must be sufciently ne to ensure that enough interfaceelements exist within the cohesive zone length at the point of crack propagation. However, for large structural models, it isalso important to avoid the computational expense of an excessively ne mesh. Therefore, mesh optimisation relies on accurate values for both cohesive zone length and the minimum number of interface elements required within this. An accurateprediction of cohesive zone length is also required in interface element fatigue degradation laws [15] .
When pioneering the use of cohesive zone models in nite element analyses of crack formation and growth in concretes,Hillerborg et al. [16] presented a characteristic length parameter ( lch ) for isotropic materials, which is a material propertygiven by the following equation:
lch E GC
r max 2 1
For the analysis of crack growth in orthotropic materials, modied versions of Eq. (1) have been developed [12,17] , which formode I and mode II loading are given by:
lch;I E 0IGIC
r I; max 2 2a
lch;II E 0IIGIIC
r II; max 2 2b
where E 0 is an equivalent elastic modulus (MPa) for orthotropic materials, whose value depends on the materials longitudinal modulus, transverse modulus, shear modulus, depth and whether plane stress or plane strain conditions exist [17] . Thisreplaces the isotropic elastic modulus in Eq. (1) . The procedure for calculating E 0 is provided in Appendix A .
Values equal to or close to the characteristic length have since been suggested by several authors [12,14,17] for predictingthe maximum numerical cohesive zone length, LCZ,f , and hence, required mesh density, in nite element analyses. The present study highlights that the characteristic length can signicantly overpredict the maximum numerical cohesive zonelength. This nding is consistent with existing analytical solutions for cohesive zone length. For example, Planas and Elices[18] have compared fully developed cohesive zone lengths in remotely loaded, isotropic, innite bodies resulting from rectilinear, linear and exponential softening tractiondisplacement laws. They found the cohesive zone length to be given by(p /8) lch , 0.731 lch and 2.92 lch for rectilinear, linear and exponential softening laws, respectively. This strong dependenceof cohesive zone length on tractiondisplacement curve shape has also been shown by Smith [19] , who developed closedform cohesive zone length solutions for a range of power law curves. One of these curves gave a close approximation of the linear softening law and similar results to those of Planas and Elices were gained.
There are several signicant differences between these analytical solutions for cohesive zone length and the presentnumerical study. All the examples quoted are based on the development of cracks in isotropic materials, but as highlightedbyYang etal. [12,17] and shown by Eqs. (2a) and (2b) , when analysing cohesivezone length in orthotropicmaterials, the elastic modulus in the characteristic length equation becomes a function of the materials longitudinal modulus, transverse modulus, shear modulus, depth and plane stress or plane strain conditions. In Turon et al.s previous study [14] , the value of E 0 wasassumed equal to the transverse modulus when predicting cohesive zone length. The present study highlights the importanceof including the additional parameters listed above in the calculation of cohesive zone length for orthotropic materials.
Furthermore, the analytical tractiondisplacement curves discussed above prescribe maximum cohesive traction at zerocrack opening displacement. However, when implementing a cohesive zone law in a numerical model, it is necessary to havean initial rising part of the tractiondisplacement curve, which is generally taken as linear to simulate the elastic response of the interface until the point of damage initiation.
Finally, the above analytical solutions are for innite bodies, where material depth has no inuence on cohesive zonelength. For analysis of composite delamination and bondline failure, it is critical that the effects of specimen thicknesson cohesive zone length are studied, due to the slender nature of typical laminates. Williams and Hadavinia [20] conductedan analytical investigation of cohesive zone models applied to a slender DCB specimen, incorporating a range of tractiondisplacement laws. Their work was motivated by developing analytical solutions for the equivalent crack length in a purelyelastic material, as opposed to the length of the cohesive zone. Based on previous studies of crack bridging models [21,22] ,Cox and Yang proposed modied forms of the characteristic length equations for innite bodies Eqs. (2a) and (2b) , whichthey suggest should be used for estimating cohesive zone length in slender laminates, with centred cracks, under mode Iand mode II loading, respectively [12] :
lch;slender ;I E 0IGIC
r I; max 2 !
14
h34 3a
lch;slender ;II
ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiE 0II;slender
GIIC
r II; max 2 !h
v uut 3b
P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792 4777
http:///?http:///? 
8/11/2019 Harper CZM
5/19
where h is the laminate halfthickness and E 0II; slender is a mode II equivalent elastic modulus for a slender body, which takes adifferent form to that used in Eq. (2b) (see Appendix A ). The mode I equivalent elastic modulus takes the same form as thatused in Eq. (2a) . These formulae are based on the assumption that the characteristic length parameter, lch , provides an accurate prediction of cohesive zone length in an innite body, which as previously discussed, is not necessarily the case. In addition, no guidance is provided concerning what constitutes a slender laminate.
No numerical studies have been presented to validate the accuracy of Eqs. (2) and (3) across a range of material properties,structural geometries and load conditions. The present paper addresses this need by investigating whether the functionalforms of these equations are applicable to numerical cohesive zone lengths and under what conditions each formula providesthe greatest level of accuracy. This is of signicant importance, both in mesh optimisation techniques for interface elementmodels, and the development of fatigue laws based on the degradation of interface elements within the cohesive zone.
With respect to the minimum number of interface elements required within the cohesive zone for an accurate failureanalysis, recommendations in the literature show a wide variation, ranging from two to more than ten [14] . Recent composite delamination analyses using interface elements have suggested that 23 elements are sufcient for mode I load cases[14,23] . This study provides a more detailed investigation, with respect to the development of the numerical cohesive zone,for mode I, mode II and mixedmode load cases.
A nal aim of the paper is to examine appropriate values of interfacial strength for modelling composite delamination.This is motivated by a technique recently demonstrated by Turon et al. [14] for reducing the required mesh density, by usinga reduction in numerical interfacial strength to increase the cohesive zone length. Such a method is very benecial fordelamination analyses involving typical composite epoxy resins, which can have cohesive zone lengths of less than 1 mmif a realistic interfacial strength is applied. As discussed above, a reduced numerical interfacial strength is allowable dueto evidence that once a crack has initiated, results are relatively insensitive to the exact value of this parameter, providedthat an accurate fracture toughness (area enclosed by the tractiondisplacement curve) is maintained. However, a previousinvestigation by Blackman et al. [9] has shown that excessively low values of interfacial strength can result in an inaccurateloaddisplacement analysis. In this case, a polynomial tractiondisplacement law was implemented, in which the interfaceelement stiffness varies prior to reaching the maximum interfacial strength (i.e. in the region 0 d e shown in Fig. 2). Whilstthe present study uses a bilinear law, in which interface element stiffness remains constant in this region, the effects of reducing interfacial strength appear consistent with those previously highlighted by Blackman et al. This suggests that limitsshould be set on allowable reductions in interfacial strength as a means of reducing the required mesh density. As for standard mesh design techniques, Turon et al.s procedure [14] relies on accurate values of numerical cohesive zone length andthe minimum number of interface elements required within this.
2. Interface element formulation
The interface elements used for this study take the form of solid hexahedral elements with a small initial thickness andare governed by a bilinear constitutive law. This was developed from a discrete interface element formulation, which hasbeen successfully implemented to model both matrix cracking and delamination within notched composites using the explicit nite element code LSDYNA [7] . Full details of the formulation are given in this previous study and so only a brief overview is now provided.
The formulation can be illustrated in a single threedimensional map, as used by several previous authors [57,24] , by representing the normal opening mode (mode I) on the 0 r d normal plane, and the transverse shear mode (mode II) on the 0 r d shear plane, as shown in Fig. 4. The triangles 0 r I,max d I,f and 0 d II,max d II,f are the bilinear responses in the pure opening andpure shear modes, respectively. Any point on the 0 d normal d shear plane represents a mixedmode relative displacement.
The mixedmode damage onset displacement, d m,e , and interfacial strength, r m,max , are calculated using a quadratic damage onset criterion:
ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffimax r I; 0
r I; max 2
r II
r II; max 2
s 1
4
The mixedmode failure displacement corresponding to complete decohesion is calculated using the following power lawfailure criterion:
GIGIC
a
GIIGIIC
a
1 5where a 2 1 : 0 2 : 0 is an empirical parameter derived from mixedmode tests, GIC and GIIC are critical energy release ratesfor pure mode I (opening) and pure mode II (shear), respectively. Eq. (5) allows the fully debonded locus, represented by therelative displacement corresponding to complete interface failure, d m,f , to be determined (see Fig. 4).
3. Benchmark applications
The baseline specimen geometry, laminate properties and interfacial properties used for the present investigation are asspecied in Fig. 5 and Table 1 . These are based on experimental data using HTA/6376C [25] , for which numerous researchers
4778 P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792
http:///?http:///? 
8/11/2019 Harper CZM
6/19
have previously conducted numerical delamination analyses under both static [26,27] and fatigue loading [15,28] . The analyses presented here have been conducted under mode I, mode II and mixedmode loading, using the DCB, 3 point endnotched exure (3ENF) and xed ratio mixedmode (FRMM) specimens, respectively. The details of each model, includingboundary conditions and properties of the numerical interface are shown in Fig. 6. It should be noted that the mode II interfacial strength of 60 MPa is signicantly higher than that of 30 MPa [15,28] and 40 MPa [26,27] applied by previous authors.As discussed in Section 4.3 , this was necessary to perform an accurate quasistatic loaddisplacement analysis of the 3ENFand FRMM specimens. Numerical results have been compared with both experimental results and corrected beam theoryresults (see Appendix B ) for the mode I and mode II load cases. Since no experimental data was available in the open literature for the mixedmode load case, only a comparison with corrected beam theory, with a set to 1 in Eq. (5) , has been made.
4. Results
4.1. Minimum number of interface elements required within the cohesive zone
As shown by Fig. 7, for the mode I DCB, the numerical cohesive zone length at the point of initial crack propagation (i.e.the crack tip interface element reaching zero traction) was measured as 1.2 mm for an element length, Lel , of 0.125 mm. Plotting a trendline through results for element lengths of 0.25 mm and 0.5 mm also provides close agreement with this value.
Referring to Fig. 8a, it is evident that all of these element lengths enable an accurate analysis of the global loaddisplace
ment response. However, the smoothness of the solution in the propagation regime decreases with increasing elementlength caused by dynamic effects as each interface element fails, due to the increasing fracture energy released by larger
B = 20mm21
3
X = 150mma 0 = 35mm
2h = 3.1mm
B = 20mm21
3
X = 150mma 0 = 35mm
2h = 3.1mm
21
3
X = 150mma 0 = 35mm
2h = 3.1mm
Fig. 5. Baseline specimen geometry.
shear
Mode II
normal
f I,
Fully debonded locus(Eqn.(5)) f m,
max II,
max I,
Damage initiationlocus (Eqn.(4))
f II,
maxm,
em,
e II,e I,
Pure Mode II  Curve(Area enclosed = G IIC )
Pure Mode I  Curve
(Area enclosed = G IC
)
m
II , II
G II in Eqn.(5)
G I in Eqn.(5)
m
II = m sin
II = m sin
I , I
I = m cos
I = m cos
shear
Mode II
normal
f I,
Fully debonded locus(Eqn.(5)) f m,
max II,
max I,
Damage initiationlocus (Eqn.(4))
f II,
maxm,
em,
e II,e I,
Pure Mode II  Curve(Area enclosed = G IIC )
Pure Mode I  Curve
(Area enclosed = G IC
)
m
II , II
G II in Eqn.(5)
G I in Eqn.(5)
m
II = m sin
II = m sin
I , I
I = m cos
I = m cos
Fig. 4. Bilinear mixedmode softening law.
Table 1
Material properties for HTA6376/C
Laminate properties Interfacial properties
E 11 (MPa) 120,000 GIC (N/mm) 0.26E 22 = E 33 (MPa) 10,500 GIIC (N/mm) 1.002G12 = G13 (MPa) 5250 r I,max (MPa) 30G23 (GPa) 3480 r II,max (MPa) 60m12 = m13 0.3 K I (N/mm 3) 1 10 5m23 0.51 K II (N/mm 3) 1 10 5
P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792 4779
http:///?http:///?http:///?http:///? 
8/11/2019 Harper CZM
7/19
elements. A global damping factor of 5 was applied in all analyses to remove high frequency oscillations whilst maintaining
accurate results. With element length increased to 1 mm, it is no longer possible to capture the cohesive zone stress distribution and the accuracy of the analysis decreases. Results become progressively worse with further reductions in mesh density (see Fig. 8b).
In the present study, the number of interface elements within the cohesive zone, N el , is dened as:
N el LCZ;f
Lel 6where LCZ,f is the length of the cohesive zone at the point of rst element failure, when using a ne mesh that enables thecohesive zone stress distribution to be accurately captured. In the present analyses, LCZ,f was measured using a 0.125 mmelement length for the DCB and FRMM specimens and a 0.25 mm element length for the 3ENF specimen. The longer elementlength used for the 3ENF specimen was possible due to the greater length of the cohesive zone.
The trends discussed above suggest that the minimum value of N el required to gain an accurate analysis of the mode I DCBspecimen lies somewhere between 1.2 and 2.4, the values calculated for element lengths of 1 mm and 0.5 mm, respectively.
This appears consistent with previous mode I studies [14,23] , which have suggested that at least two elements are requiredwithin the cohesive zone for an accurate global loaddisplacement analysis.
Fig. 6. Finite element models for the benchmark load cases.
4780 P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792

8/11/2019 Harper CZM
8/19
Fig. 8. DCB loaddisplacement curves in relation to the number of interface elements within the numerical cohesive zone.
0
5
10
15
20
25
30
35
0 0.2 0.4 0.6 0.8 1 1.2 1.4
Distance from numerical crack tip (mm)
M o
d e
I S t r e s s
( M P a
)
I,max
LCZ,f for elementlength of 0.125mm
0.125mm0.25mm0.5mm
Element Length
Fig. 7. Cohesive zone stress distribution for DCB model at point of rst element failure.
P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792 4781

8/11/2019 Harper CZM
9/19
Similar results are exhibited for the 3 point ENF and FRMM specimens ( Figs. 912 ). In the case of the 3 point ENF, whichhas a numerical cohesive zone length of 4.1 mm (see Fig. 9), there is a signicant reduction in the accuracy of results whenincreasing element length from 1.5 mm to 2 mm. For an element length of 1.5 mm, results show close agreement with thoseobtained using ner meshes. When element length is increased to 2 mm, the model fails to accurately capture the point of propagation and there are signicant oscillations present in the propagation regime. This suggests that the minimum valueof N el for an accurate analysis lies somewhere between 2.05 and 2.73. ( NB: results for the nest mesh used for the 3ENF, withan element length of 0.25 mm, have not been displayed on Fig. 9 and 10 because, due to the long cohesive zone length, theyshow no signicant variation from those for an element length of 0.5 mm).
For the FRMM specimen, which has a numerical cohesive zone length of 1.5 mm, analysis accuracy deteriorates when element length is increased from 0.5 mm to 1 mm. This indicates that the minimum value of N el lies between 1.5 and 3.
Although further work remains to precisely dene a minimum required N el for accurate numerical analyses under variousmode ratios, a conservative approach would be to require that N el P 3. This will ensure that the cohesive zone stress distribution at the point of rst element failure is correctly captured, hence preventing delayed propagation onset.
4.2. Cohesive zone length
Since equations for estimating cohesive zone length are dependent on E 0, GC, r max and h (see Eqs. (2) and (3) ), their effectson the fully developed numerical cohesive zone length, LCZ,f , have been investigated. Fig. 13 shows the effects on LCZ,f of independently varying these parameters for the benchmark HTA6376/C mode I DCB model, using a consistent element length of 0.125 mm. ( NB: as shown in Appendix A , E 0 is inuenced by E 11 , E 33 and G13 , therefore, each of these parameters has beenindependently varied). Due to the uncertainties surrounding the accuracy of existing predictive formulae highlighted inthe introduction, a scaling factor, M , has been applied to Eqs. (2) and (3) , to try and identify the best t to numerical results.
0
10
20
30
40
50
60
70
0 0.5 1 1.5 2 2.5 3 3.5 4 4.5 5
Distance from numerical crack tip (mm)
M
o d e
I I S t r e s s
( M P a
) II,max
0.5mm1mm1.5mm
Element Length
LCZ,f for elementlength of 0.5mm
Fig. 9. Cohesive zone stress distribution for 3ENF model at point of rst element failure.
Fig. 10. 3ENF loaddisplacement curves for a range of element lengths.
4782 P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792
http:///?http:///? 
8/11/2019 Harper CZM
10/19
When comparing the numerical results with Eqs. (2a) and (3a) (i.e. the characteristic cohesive zone lengths, lch,I andlch,slender,I , in innite and slender bodies, respectively), it was apparent that both formulae signicantly overpredict thenumerical cohesive zone length. As a result, using these formulae for mesh design risks the application of a mesh thatis too coarse to accurately model failure. It was identied that applying M = 0.5 to Eq. (3a) , which accounts for the inuence of specimen depth, provides a reasonable and generally conservative correlation with the numerical results acrossmost of the parameter ranges investigated. In cases where material properties result in a very short cohesive zone length(e.g. high interfacial strength, low shear modulus, low transverse modulus), Eq. (2a) , which takes no account of structuraldepth, begins to exhibit a closer match to the numerical results. Again, it is necessary to use M = 0.5 in order to gain a closematch with the numerical results. It is apparent that this value falls between the analytical solutions for cohesive zonelengths in innite bodies of M = p /8 and M = 0.731, for rectilinear and linear softening tractiondisplacement laws, respectively [18] . Eqs. (2a) and (3a) , with a scaling factor of M = 0.5 applied, have been plotted on Fig. 13 to highlight the trendsdiscussed.
Very similar observations can be made for the mode II cohesive zone length results shown in Fig. 14 , for an element lengthof 0.25 mm. Again, Eq. (3b) , which accounts for structural depth, generally provides the best correlation with numerical results, but it is necessary to apply M = 0.5 to gain a close match. Previous work by Massabo and Cox [22] has shown that theequivalent mode II modulus in the characteristic length equation for slender bodies, E 0II; slender , takes the same value as the lon
gitudinal modulus, E
11 , and is inuenced by no other elastic moduli. However, the cohesive zone length in the 3ENF specimen is seen to increase from a value of 3 mm for a shear modulus, G13 , of 1000 MPa to 4.3 mm for a shear modulus, G13 , of
0
10
20
30
40
50
60
70
0 0.25 0.5 0.75 1 1.25 1.5 1.75
Distance from numerical crack tip (mm)
M i x e
d M o d e
S t r e s s
( M P a
)
LCZ,f for elementlength of 0.125mm
0.125mm0.25mm
0.5mm
Element Length
max
Fig. 11. Cohesive zone stress distribution for FRMM model at point of rst element failure.
Fig. 12. FRMM loaddisplacement curves for a range of element lengths.
P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792 4783

8/11/2019 Harper CZM
11/19
7000 MPa. Therefore, whilst the inuence of shear modulus is relatively weak compared to that of longitudinal modulus, itcannot be neglected. This highlights the difculty in drawing a clear distinction between what constitutes a slender or innite body. Relative to the mode I load case, the cohesive zone lengths for mode II are signicantly longer. As suggested byprevious authors [12] , this highlights that for typical composite material properties, it will generally be the mode I cohesivezone length that dictates the minimum mesh density.
In order to investigate the accuracy of Eqs. (2) and (3) in situations where the structural depth has a less signicant inuence, an additional mode I DCB model was created, using the specimen geometry and material properties shown in Table 2 .This is based on data provided in reference [14] for a T300/9772 specimen, which has a signicantly increased mode I fracture toughness, GIC (+74%), interfacial strength, r I,max (+200%), specimen depth, h (+32%), initial crack length, a0 (+57%), andlongitudinal modulus, E 11 (+25%), relative to the HTA/6376C specimen. A consistent element length of 0.125 mm was againused.
Fig. 15 highlights that for these material properties, the specimen depth has a much less signicant inuence across therange of parameters investigated and Eq. (2a) frequently gives a more accurate prediction of numerical cohesive zone lengththan Eq. (3a) . Again, it is necessary to apply M = 0.5 to gain a close match to the numerical results. Only for cases where thevariation of a material property signicantly extends the cohesive zone length, such as reduced interfacial strength or in
creased fracture toughness, does Eq. (3a) provide the best correlation. It is always the minimum of the two analytical values,provided by Eqs. (2a) and (3a) , respectively, which provides the closest match to numerical results.
0
0.5
1
1.5
2
2.5
3
0 10000 20000 30000 40000 50000
E33 (MPa)
L C Z
, f ( m m
)
00.5
1
1.5
2
2.5
3
0 0.2 0.4 0.6 0.8 1G IC (N/mm)
L C Z
, f ( m m
)
00.5
1
1.5
2
2.5
3
0 10 20 30 40 50 60 70 I,max (MPa)
L C Z
, f ( m m
)
0
0.5
1
1.5
2
2.5
3
0 0.5 1 1.5 2 2.5
h (mm)
L C Z
, f ( m m
)
0
0.5
1
1.5
2
2.5
3
0 50000 100000 150000 200000
E 11 (MPa)
L C Z
, f ( m m
)
0
0.5
1
1.5
2
2.5
3
0 2000 4000 6000 8000
G13 (MPa)
L C Z
, f ( m m
)
Numerical )a3.( Eqn5.0 L f ,CZ =)a2.( Eqn5.0 L f ,CZ =
Fig. 13. Effect of material properties and depth on mode I cohesive zone length for the HTA6376/C benchmark DCB model.
4784 P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792

8/11/2019 Harper CZM
12/19
Numerical )b3.( Eqn5.0 L f ,CZ =)b2.( Eqn5.0 L f ,CZ =
0
12345678
0 10000 20000 30000 40000 50000
E33 (MPa)
L C Z
, f ( m m
)
01
2
3
4
5
6
7
8
0 0.5 1 1.5 2 2.5
G IIC (N/mm)
L C Z
, f ( m m
)
01
2
3
4
5
6
7
8
50 60 70 80 90 100 110 120 130
II,max (MPa)
L C Z
, f ( m m
)
0
1
2
3
4
5
6
7
8
0.5 1 1.5 2 2.5
h (mm)
L C Z
, f ( m m
)
0
1
2
3
4
5
6
7
8
0 50000 100000 150000 200000
E11 (MPa)
L C Z
, f ( m m
)
0
12
345
678
0 2000 4000 6000 8000
G13 (MPa)
L C Z
, f ( m m
)
Fig. 14. Effect of material properties and depth on mode II cohesive zone length for the HTA/6376C benchmark 3ENF model.
Table 2
Material and geometric properties for T300/9772 DCB model
Laminate properties Interfacial properties
E 11 (MPa) 150,000 GIC (N/mm) 0.352E 22 = E 33 (MPa) 11,000 r I,max (MPa) 60G12 = G13 (MPa) 6000 GIIC (N/mm) 1.002G23 (MPa) 3700 r II,max (MPa) 60m12 = m13 0.3 K I (N/mm 3) 1 10 5m23 0.51 K II (N/mm 3) 1 10 5
Geometric properties X (mm) 150 h (mm) 1.98a0 (mm) 55 B (mm) 20
NB: The poisson ratios ( m12 , m13 , m23 ), mode II interfacial properties ( GIIC, r II,max , K II) and mode I interfacial stiffness ( K I) shown in Table 2 are identical to thoseapplied for the HTA/6376C specimen. All other properties are consistent with those shown in reference [14] for a T300/9772 mode I DCB specimen.
P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792 4785

8/11/2019 Harper CZM
13/19
The cohesive zone length results for both the mode I and mode II load cases suggest that a reasonable match to thenumerical results is always obtained by applying M = 0.5 to the minimum value from Eqs. (2) and (3) . Further work remainsto investigate appropriate values of M for alternative tractiondisplacement laws and for a wider range of crack lengths andstructural geometries.
Combining these results with those discussed in Section 4.1 , the proposed mesh design strategy for a general mixedmodeload case, when using a bilinear tractiondisplacement law, is as follows:
(i) Predict the minimum possible length of the fully developed cohesive zone, LCZ,f,predicted , using the formula,
LCZ;f ;predicted 0:5min Eqn: 2a; 2b; 3a; 3b 7Based on the cohesive zone results presented in Figs. 1315 , the only case where this formula risks providing a signicant overprediction of cohesive zone length is when the transverse modulus, E 33 , has a value above
12,000 MPa. This is apparent from Fig. 15, where the numerical cohesive zone length for the T300/9772 DCB modelshows a maximum variation of 30% below that predicted by Eq. (3a) with a scaling factor of M = 0.5 applied.
0
0.5
1
1.5
2
0 0.2 0.4 0.6 0.8 1
G IC (N/mm)
L C Z
, f ( m m
)
0
0.5
1
1.5
2
20 30 40 50 60 70 80
I,max (MPa)
L C Z
, f ( m m
)
0
0.5
1
1.5
2
0 0.5 1 1.5 2 2.5
h (mm)
L C Z
, f ( m m
)
0
0.5
1
1.5
2
0 10000 20000 30000 40000 50000
E33 (MPa)
L C Z
, f ( m m
)
0
0.5
1
1.5
2
0 50000 100000 150000 200000
E11 (MPa)
L C Z
, f ( m m
)
0
0.5
1
1.5
2
0 2000 4000 6000 8000 10000
G 13(MPa)
L C Z
, f ( m m
)
Numerical )a3.( Eqn5.0 L f ,CZ =)a2.( Eqn5.0 L f ,CZ =
Fig. 15. Effect of material properties and depth on mode I cohesive zone length for a T300/9772 DCB model.
4786 P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792
http:///?http:///? 
8/11/2019 Harper CZM
14/19
(ii) Divide this result by 3 to calculate the maximum allowable element length, Lel,max , in order to ensure that at least threeinterface elements are present within the fully developed cohesive zone:
Lel; max LCZ;f ;predicted
3 : 8
4.3. Effects of varying Numerical Interfacial Strength
Figs. 1618 show the effects of varying mode I and mode II interfacial strength on the loaddisplacement analyses of thebenchmark DCB, 3ENF and FRMM specimens. For each specimen, results are presented in the following forms:
(i) Using a ne mesh, which enables the cohesive zone stress distribution to be accurately captured for all values of numerical strength investigated. The fully developed cohesive zone length, LCZ,f , for each value of interfacial strengthis also shown so that the accuracy of the analyses can be related to this parameter.
(ii) Using a coarse mesh, where the number of elements within the cohesive zone is initially less than the minimumrequired value, when applying the baseline interfacial strength (see Section 4.1 ). This enables allowable reductionsin interfacial strength to be investigated, when using this technique to reduce the minimum required mesh density,as originally proposed by Turon et al. [14] .
In Fig. 16a, mode I interfacial strength is reduced from 45 MPa (15 MPa above the baseline value) to 5 MPa for the DCBspecimen, using a ne mesh with an element length of 0.125 mm. Between 45 MPa and 30 MPa there is no signicant change
Fig. 16. Effect of numerical interfacial strength variation on mode I DCB model (HTA/6376C).
P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792 4787
http:///?http:///? 
8/11/2019 Harper CZM
15/19
in the accuracy of the numerical analysis and both loaddisplacement curves show close agreement with corrected beamtheory. From 30 MPa to 10 MPa, there is a gradual loss of stiffness in the elastic loading regime prior to crack propagation,but this is reasonably small in magnitude and does not produce a large deterioration in analysis accuracy. When the numerical interfacial strength is decreased from 10 MPa to 5 MPa and the cohesive zone length increases from 3.25 mm to 6 mm, amuch larger deterioration in stiffness occurs and the point of crack propagation is signicantly delayed. Fig. 16b shows theeffects of reducing mode I interfacial strength for a coarse mesh of 1 mm element length, which is unable to accurately capture the cohesive zone distribution at the point of rst element failure when using the baseline value of 30 MPa (see Fig. 8b).As interfacial strength is reduced, the same trends as those discussed for the ne mesh regarding loss of stiffness in the elastic regime are apparent. However, signicant improvements in analysis accuracy in the propagation regime are gained due toan increased number of elements within the cohesive zone at the point of rst element failure.
Fig. 17 a shows the effects of varying interfacial strength for the 3ENF specimen, using a ne mesh with an element lengthof 0.25 mm. It is evident that for a mode II interfacial strength of 30 MPa, as applied by previous authors [15,28] , the analysiscannot accurately capture the peak load prior to crack propagation. This is due to a signicant loss of stiffness during theelastic loading regime. However, with interfacial strength increased to a more realistic value of 60 MPa, a much closer matchto the corrected beam theory solution is obtained. No signicant further improvement is gained by increasing interfacialstrength to 90 MPa. This justies the value of 60 MPa selected for the numerical mode II interfacial strength in the baselinemodel. The poor results gained using lower values of interfacial strength are believed to be due to the very long numericalcohesive zone lengths (10.5 mm for 30 MPa and 20.25 mm for 15 MPa) and hence signicant softening ahead of the crack tip.Fig. 17 b shows the effects of reducing interfacial strength using a coarse mesh with an element length of 2 mm. This elementlength is greater than that of 1 mm used for the DCB due to the longer cohesive zone length resulting from the baselinematerial properties. This means that for the 3ENF model, it is only when element length is increased from 1.5 mm to
Fig. 17. Effect of numerical interfacial strength variation on mode II 3ENF model (HTA/6376C).
4788 P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792

8/11/2019 Harper CZM
16/19
2 mm that there becomes an insufcient number of elements within the cohesive zone to accurately capture the point of crack propagation (see Fig. 10). As for the DCB, reduced interfacial strength increases the accuracy of the analysis in the propagation regime. However, comparison with Fig. 17a shows that the initial point of crack propagation for a ne mesh cannotbe regained. This is likely to be due to the coarseness of the mesh combined with the very sudden nature of crack propagation in the 3ENF specimen.
Fig. 18 a shows the effects of reducing mode I and mode II interfacial strengths in equal proportions below their baselinevalues for the FRMM specimen, when using a ne mesh with an element length of 0.125 mm. The cohesive zone lengthsexhibited for each combination of mode I and mode II interfacial strength appear to be dictated mainly by the mode I value.This explains why, similar to the mode I DCB, a signicant loss in stiffness within the elastic regime only occurs when mode Iinterfacial strength is reduced below 10 MPa and the cohesive zone length exceeds approximately 5 mm. Fig. 18b shows theeffects of reducing mode I and mode II interfacial strengths, for a coarse mesh of 1 mm element length, which is unable tocapture the cohesive zone distribution at the point of rst element failure when using the baseline values of 30 MPa and60 MPa, respectively (see Fig. 12). Similar to results for the mode I DCB, signicant improvements in analysis accuracy withinthe propagation regime are obtainable with reduced interfacial strength but at the expense of reduced stiffness in the elasticregime.
The above ndings indicate that care must be taken when reducing interfacial strength as a means of reducing the required mesh density in numerical models. For typical carbon epoxy properties, a very short mode I cohesive zone lengthexists, allowing signicant reductions in mode I interfacial strength, without affecting the accuracy of global loaddisplacement analyses. However, mode II cohesive zone lengths are generally much longer, and similar mode II interfacial strengthreductions can result in signicant inaccuracies. Further investigation is required to provide a denitive value for the extentto which interfacial strength can be reduced in relation to numerical cohesive zone length, whilst preserving analysis
Fig. 18. Effect of numerical interfacial strength variation on FRMM model (HTA/6376C).
P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792 4789

8/11/2019 Harper CZM
17/19
accuracy, for a range of crack lengths. For the cases discussed above, a signicant loss of stiffness in the elastic regime of theloaddisplacement curve is evident when the fully developed cohesive zone length exceeds approximately 5 mm.
5. Conclusions
The present study has shown that a minimum of between two and three elements need to be present within the numerical cohesive zone for an accurate load displacement analysis to be performed under mode I, mode II and mixedmode load
cases. This is necessary for an accurate representation of the numerical stress distribution within this zone at the point of initial crack propagation.A clear distinction has been drawn between the physical cohesive zone length, the analytical cohesive zone length and
that which results from a numerical representation using interface elements. For the rst time, the length of the numericalcohesive zone has been investigated in detail and compared to closed form solutions across a range of material and geometric parameters. It has been demonstrated that using a bilinear tractiondisplacement curve, many current analytical formulae for cohesive zone length signicantly overpredict numerical values. In addition, parameters not always included incurrent formulae for predicting cohesive zone length, such as specimen depth, longitudinal modulus and shear modulus,are shown to have a signicant inuence in slender, orthotropic materials. These ndings have important implications inmesh design methods, which rely on an accurate prediction of cohesive zone length to minimise computational expense,whilst preserving the accuracy of numerical analyses. Modications to existing formulae have been proposed for predictingcohesive zone length in standard fracture toughness tests, but they remain to be validated in more complex structural geometries. Their applicability to alternative types of tractiondisplacement response, such as exponential and trapezoidal forms,
also requires investigation.It has been demonstrated that although reductions in numerical interfacial strength can be used to increase the cohesivezone length and reduce the required mesh density, limits exist on the allowable magnitude of these reductions. For typicalcarbon epoxy composite properties, the mode I cohesive zone length is generally very short, and signicant reductions inmode I interfacial strength are possible, without affecting the accuracy of global loaddisplacement analyses. However, comparable reductions in mode II interfacial strength can cause excessive material softening ahead of the crack tip, due to thedevelopment of extremely long cohesive zones. This results in failure to predict the peak load at which initial crack propagation occurs in global loaddisplacement analyses.
Acknowledgements
The authors would like to thank Leif Asp and Rikard Borg for their help in supplying experimental data, against which theanalytical and numerical results gained in this study have been compared.
Appendix A. Calculation of elastic modulus for cohesive zone length equations
The elastic constant E 0 that appears in Eqs. (2a), (2b), (3a) and (3b) is dependent on the mode of loading, whether planestress or plane strain conditions exist and whether the specimen can be considered as slender or innite.
For a mode I crack in an innite body under plane stress conditions [17] :
1E 0I ffiffiffiffiffiffiffiffiffiffiffiffiffi ffib11 b332r ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffib33b11
1=2
2b31 b55
2b11s A:1where the b ij are Voigt elastic constants dened by:
ei
X
6
j
1
bijr j; A:2with e1 e11 , . . .,e6 e 12 ; r 1 r 11 , . . ., r 6 r 12 . For a specially orthotropic specimen (axes of orthotropy aligned with theaxes of symmetry of the specimen), the Voigt elastic constants are related to the engineering elastic constants by:
b11 1=E 11 ; b12 m12 =E 11 ; b66 1=G12 ;b22 1=E 22 ; b23 m23 =E 22 ; b55 1=G31 ;b33 1=E 33 ; b31 m31 =E 33 ; b44 1=G23 ;
A:3
where E ii is the Youngs modulus in the xi direction, mij is a Poissons ratio and Gij is an engineering shear modulus. For thealignment of the specimen in Fig. 5, the engineering constants involved in E 0I are E 11 , E 33 , G31 and m31 .
For a crack in an innite body that is loaded in shear, the elastic constant becomes:
1E 0II
ffiffiffiffiffiffiffiffiffiffiffiffib11 =2
q ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffib11 b33
1=2
b31 b55 =2
q A:4
4790 P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792

8/11/2019 Harper CZM
18/19
In a slender body, a different elastic constant appears. For example, in a thin plate or beam containing a midplane crackpropagating in the x1 direction and loaded in mode II, the elastic constant that appears in results for the cohesive zone lengthis the reduced Youngs modulus:
E 0II;slender E 11
1 m13 m31 A:5
Appendix B. Corrected beam theory equations
B.1. Mode I DCB
Considering the DCB specimen (see Fig. 6a) as two single cantilever beams, of length equal to the crack length, a , simplebeam theory can be applied to give:
DI 2Pa3
3E 11 I B:1where D I = vertical separation of cantilever beam tips; P = point load applied to the free end of each cantilever; E 11 = Youngsmodulus of each cantilever along its length; and I = second moment of area of each cantilever (= Bh3/12, where B and h are thespecimen width and halfdepth, respectively, as dened in Fig. 5).
In order to correct the displacement for shear deformation and for local deformations that occur around the crack tip, a
corrected beam theory method can be used, in which Eq. (B.1) becomes:
DI 2P a vh
3
3E 11 I B:2where v = correction parameter; and h = cantilever depth.
A value of v can be determined both experimentally and analytically, but in this study, the analytical value presented byReeder et al. is used [29] , where:
v ffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiffiE 1111 G13 32 C1 C 2" #v uut
B:3aand
C 1:18 ffiffiffiffiffiffiffiffiffiffiffiffiffiffiE 11 E 22p G13 B:3b
The mode I strain energy release is given by [29] :
GI P 2a vh
2
BE 11 I B:4Under a linearly increasing tip displacement, the load ( P ) increases until the point where GI = GIC and the crack begins topropagate. The subsequent loaddisplacement relationship for each increment of crack extension is found by combiningEqs. (B.2) and (B.4) with GI set equal to GIC.
B.2. 3 Point ENF
The same principles apply for the 3 point ENF (see Fig. 6b), in which the displacement and mode II strain energy releaserate before initial crack propagation are given by [29] :
DII 3P a 0:42 vh
3
2PL3
96 E 11 I B:5
GII 3a 0:42 vh
2P 2
64 BE 11 I B:6NB: the second moment of area, I , in Eqs. (B.5) and (B.6) remains equal to that calculated for the DCB specimen, using half thespecimen depth and the length, L, is as dened in Fig. 6b.
B.3. FRMM
For the FRMM specimen (see Fig. 6c), the upper cantilever tip displacement and separate mode I and mode II strain energyrelease rate components are given by [30] :
P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792 4791

8/11/2019 Harper CZM
19/19
D PN 07a 0:42 vh
3
L 2vh3
2Bh3 E 11 B:7
GI 3FP 2a vh
2
B2h3E 11 B:8
GII 9FP 2
a
0:42 vh
2
4B2 h3 E 11 B:9where F and N 0 are correction factors for large displacements and the length, L, is as dened in Fig. 6c. Due to the small displacement of approximately 3 mm at the point of initial crack propagation, F and N 0 have been assumed equal to unity for theFRMM specimen used in this study. Under a linearly increasing upper cantilever tip displacement, the analytical load, P , atwhich initial crack propagation occurs was calculated using the power law failure criterion given by Eq. (5) , with a = 1.
References
[1] Mi Y, Criseld MA, Davies GAO, Hellweg HB. Progressive delamination using interface elements. J Compos Mater 1998;32:124672.[2] Petrossian Z, Wisnom MR. Prediction of delamination initiation and growth from discontinuous plies using interface elements. Compos A: Appl Sci
Manufactur 1998;29A:50315.[3] Chen J, Criseld M, Kinloch AJ, Busso EP, Matthews FL, Qiu Y. Predicting progressive delamination of composite material specimens via interface
elements. Mech Compos Mater Struct 1999;6:30117.[4] Criseld MA, Alfano G. Finite element interface models for the delamination analysis of laminated composites: mechanical and computational issues.
Int J Num Meth Eng 2000;50:170136.[5] Camanho PP, Davila CG, De Moura MF. Numerical simulation of mixedmode progressive delamination in composite materials. J Compos Mater
2003;37:141524.[6] Pinho ST, Ianucci L, Robinson P. Formulation and implementation of decohesion elements in an explicit nite element code. Compos A: Appl Sci
Manufactur 2006;37:77889.[7] Jiang WG, Hallett SR, Green BG, Wisnom MR. A concise interface constitutive law for analysis of delamination and splitting in composite materials and
its application to scaled notched tensile specimens. Int J Num Meth Eng 2007;69:198295.[8] Camanho PP, Davila CG, Pinho ST. Fracture analysis of composite cocured structural joints using decohesion elements. Fatigue Fract Eng Mater Struct
2003;27:74557.[9] Blackman BRK, Hadavinia H, Kinloch AJ, Williams JG. The use of a cohesive zone model to study the fracture of bre composites and adhesivelybonded
joints. Int J Fract 2003;119:2546.[10] Li S, Thouless MD, Waas AM, Schroeder JA, Zavattieri PD. Mixedmode cohesivezone models for fracture of an adhesively bonded polymermatrix
composite. Eng Fract Mech 2006;73:6478.[11] Goyal VK, Johnson ER, Goyal VK. Predictive strengthfracture model for composite bonded joints. Compos Struct 2008;82:43446.[12] Cox B, Yang Q. Cohesive models for damage evolution in laminated composites. Int J Fract 2005;133:10737.[13] Shet C, Chandra N. Effect of the shape of tractiondisplacement cohesive zone curves on the fracture response. Mech Adv Mater Struct
2004;11:24975.[14] Turon A, Davila CG, Camanho PP, Costa J. An engineering solution for mesh size effects in the simulation of delamination using cohesive zone models.
Eng Fract Mech 2007;74:166582.[15] Turon A, Costa J, Camanho PP, Davila CG. Simulation of delamination in composites under highcycle fatigue. Compos A: Appl Sci Manufactur
2007;38:227082.[16] Hillerborg A, Modeer M, Petersson PE. Analysis of crack formation and growth in concrete by means of fracture mechanics and nite elements. Cement
Concrete Res 1976;6:77382.[17] Yang QD, Cox BN, Nalla RK, Ritchie RO. Fracture length scales in human cortical bone: the necessity of nonlinear fracture models. Biomaterials
2006;27:2095113.[18] Planas J, Elices M. Nonlinear fracture of cohesive materials. Int J Fract 1991;51:13957.[19] Smith E. The effect of the stressrelative displacement law on failure predictions using the cohesive zone model. Int J Fract 1999;99:4151.[20] Williams JG, Hadavinia H. Analytical solutions for cohesive zone models. J Mech Phys Solids 2002;50:80925.[21] Bao G, Suo Z. Remarks on crackbridging concepts. Appl Mech Rev 1992;24:35566.[22] Massabo R, Cox BN. Concepts for bridged mode II delamination cracks. J Mech Phys Solids 1999;47:1265300.[23] Barua A, Bose K. On the optimum choices of cohesivezone parameters describing initiation and propagation of cracks. In: ECCOMAS thematic
conference on mechanical response of composites, Porto, Portugal; September 2007. p. 124.[24] Hallett SR, Wisnom MR. Modelling and experimental investigation of progressive damage in notched composites. In: 17th American society for
composites technical conference, West Lafayette; 2002.[25] Asp LE, Sjogren A, Greenhalgh ES. Delamination growth and thresholds in a carbon/epoxy composite under fatigue loading. J Compos Technol Res
2001;23:5568.[26] Borg R, Nilsson L, Simonsson K. Modelling of delamination using a discretized cohesive zone and damage formulation. Compos Sci Technol
2002;62:1299314.[27] Borg R, Nilsson L, Simonsson K. Simulating DCB, ENF and MMB experiments using shell elements and a cohesive zone model. Compos Sci Technol
2004;64:26978.[28] Robinson P, Galvanetto U, Tumino D, Belluci G. Numerical simulation of fatiguedriven delamination using interface elements. Int J Num Meth Eng
2004;63:182448.[29] Reeder JR, Demarco K, Whitley KS. The use of doubler reinforcement in delamination toughness testing. Compos A: Appl Sci Manufactur
2004;35:133744.[30] Kinloch AJ, Wang Y, Williams JG, Yayla P. The mixedmode delamination of bre composite materials. Compos Sci Technol 1993;47:22537.
4792 P.W. Harper, S.R. Hallett / Engineering Fracture Mechanics 75 (2008) 47744792